The effect of duration of finishing and polishing on the surface
roughness of two composite resins
Received: 24/11/2011 Accepted: 29/7/2012
Razawa K. Saeed * Media A. Saeed * Intesar S. Toma *
Background and objective: The purpose of this study was to evaluate the effect of duration of finishing and polishing procedures on the surface roughness of two different types of composite resins.
Methods: Forty samples of 6 mm in diameter and 2 mm in depth were prepared, 2 types of composite resins were used (nanocomposite and hybrid composite resin). Twenty samples of each type of material were prepared and divided into two main groups and then each main group subdivided randomly into two subgroups of 10 samples for each subgroup (one). Ten samples of each material were submitted to finishing by using a finishing kit. The available finishing kits used in this study containing discs, cups and points that were used with a slow-speed hand piece in a dry field and with a light intermittent pressure for about 15 seconds. While the other 10 samples of each material were finished for about 30 second; then the analysis of the surface roughness was carried out, three readings were made on each surface using a stylus tip and the extension of each reading was 2 mm stroke.
Results: There was non significant difference between the groups that were finished and polished for 15 second and the other groups that were finished and polished for 30 second for the two different types of composite resin.
Conclusion: Increasing duration of finishing and polishing has no effect on the surface
roughness ofThe two different types of composite resin.
Keywords: Nano composite, Hybrid composite, Finishing bur, Duration. Abstract
* Department of Conservative Dentistry, College of Dentistry, Hawler Medical University, Erbil, Iraq. Introduction
The timing of the finishing/polishing proce-dure might have an effect on the physical properties of the restorative materials, and
might increase the risk of premature failures. Although several authors have
proposed a 24-hour delay before the completion of finishing procedures, most
clinicians perform finishing/polishing procedures immediately after restoration
placement 1. There was a need for a highly
polishable composite resin with optimal physical properties for use in the anterior
and posterior regions 2. Composite resin
restorations have evolved rapidly, with the pace of new product development
acceler-ating over the last decade. Advanced composite materials and techniques, new etching and bonding materials, fast curing
lights, and new finishing and polishing materials and techniques have all been
introduced 3. As a consequence,
irregulari-ties appear on the surface of the restora-tions. The filler content of the composite resin also affects roughness; similarly, the resin matrix composition may also play a role in the final smoothness of the
restora-tion 4. A smooth surface on a restoration
can be obtained after polymerizing the resin composite against an appropriate
matrix strip, but further countering and finishing are required to remove excess
material and to obtain a smooth glossy
surface 5. Minimizing finishing and
minimize the need for subsequent finishing. The ideal direct resin restoration would require no finishing or polishing once completed. Since most operative conditions
are less than ideal, minor finishing requirements must be addressed. Various
instruments (e.g. diamond burs, carbide burs, polishing disks, diamond-impregnated rubber points, polishing pastes) are avail-able for sequential finishing and
polish-ing5,13. The presence of surface
irregulari-ties arising from poor polishing can create clinical problems such as gingival irritation,
surface staining, plaque accumulation and
secondary caries 3. However, the durability
of the smoothness is difficult to predict and may be influenced by factors related both to the clinical restorative procedure and to the composition of the material, especially the filling particle size 14, 15.
Forty samples were prepared by cutting a pvc pipe (Pvc pipe, Jordan) 2.5 cm in diameter and 2 cm in height with a hot knife and then pouring each plastic tube which is 2.5 cm in diameter and 2cm in height with cold cure acrylic resin (MR, dental, UK) and then cylindrical cavities 6 mm in diameter and 2 mm in depth were cut at the center of cold cure acrylic resin blocks, by placing a metal mold on the acrylic resin at the dough stage of setting of acrylic resin and the excess of acrylic was removed by wax knife before setting and after setting of acrylic resin the metal mold is removed. Two types of composite resins were used (Composan bio-esthetic nano particles composite resin (Promedica, Germany) and Composan ceram hybrid composite
resin (Promedica, Germany)).Twenty samples of each type of material were prepared, specimens were divided by simple random method into 2 groups;
Group A: 20 samples of nanocomposite, Group B: 20 samples of hybrid composite. Then each group was subdivided randomly
into 2 subgroups; 1. 10 finished and
polished for 15 seconds 16 2.10 finished
and polished for 30 seconds 17. Composite
was inserted into the mold in one incre-ment with aplastic instruincre-ment; a celluloid strip (Hawe transparent strips) and a glass slab were placed over the composite resin
under the load of 200 gm 14, 18 to remove
excess material, then after removal of the glass slab the sample were light cured by
halogen light curing (Dentsply, USA) device for 40 second according to
manu-facturer instructions between all steps of the procedure, the samples were stored in distilled water in an incubator at 37C 18, 19.
Ten samples of each material were submit-ted to finishing and polishing by using an ivoclar viva dent finishing kit. The available finishing kits used in this study containing discs, cups and points that used with a slow-speed hand piece in a dry field and with a light intermittent pressure (to avoid the build-up of heat on the material as well as deterioration of the finishing material) for about 15 second. While the other ten samples of each material were finished for about 30 second; then the analysis of the surface roughness was carried out. All specimens were individually positioned in a surface recorder profilometer to verify the roughness (Ra) values of the material surface, three readings were made on each surface using a stylus tip, and the extension of each reading was 2 mm stroke.
By using paired t- test, the result revealed that there was non significant difference
between the groups of finishing and polishing of 15 seconds and groups of finishing and polishing of 30 but generally the groups that have been finished and polished for 30 seconds shows a smoother surface if compared to groups that have been finished and polished for 15 seconds however the difference was non significant at p> 0.05, Table 1, 2 and Figure 1, and there was non significant difference be-tween the two different materials (nano composite and hybrid composite). But gen-erally the nano fill composite groups have smoother surface at both 15 and 30 Methods
Types of composite resin Duration of finishing and polishing No. of samples Mean of Ra in Mm SD Std. Error Mean
Nano-fill composite resin 15 second 10 0.338 ± 0.071 0.022
Micro hybride composite
resin 15 second 10 0.410 ± 0.159 0.050
Nano-fill composite resin 30 second 10 0.307 ± 0.051 0.016
Micro hybride composite
resin 30 second 10 0.358 ± 0.086 0.027
Table 2: t-test for difference between the groups in the duration of finishing and
polishing Table3: t-test for difference between the
groups in the filler contain of composite
Technique df t-statistic P-value Sign.
Finishing for 15 and 30 seconds of nano composite
18 1.123 0.276 NS
Finishing for 15 and 30 seconds of micro-hybride composite
18 1.912 0.374 NS
Technique df t-statistic P-value Sign.
15 second 18 -1.307 0.208 NS
for30 second 18 -1.616 0.124 NS
Figure 1: Bar chart for the surface roughness study results for duration of finishing and polishing of two composites.
ite resin groups at both duration but the difference was non significant at p> 0.05 ,Table 3.
seconds duration of finishing and polishing if compared to the micro hybride
Finishing and polishing of resin composite restorations are steps critical to enhancing the esthetic and longevity of restored teeth
20.Finishing refers to gross contouring or
reducing of the restoration to obtain the desired anatomy. Polishing reduces the roughness and scratches created by finish-ing instruments. Rough, poorly polished surfaces contributed to staining, plaque accumulation, gingival irritation and
recur-rent caries 21. The factors determining the
micro morphology of the surface composite
resin restorations after finishing and polishing include composite characteristics
such as size, hardness, type and amount of particles and factors related to the abrasive system such as flexibility of the material in
which the abrasive is impregnated, hardness of the abrasive, and geometry,
speed and form of application of the
instruments used 22. Finishing and
polish-ing procedures require sequential use of instrument with gradual decrease in particles abrasiveness, aiming to obtaining
a brighter and smoother surface 20.This
study sought to investigate the influence of
duration of finishing and polishing on the surface roughness of Composan bio-esthetic nano particles composite resin
and Composan ceram hybrid composite resin. The results revealed that Composan bio-esthetic nano composite finished with finishing kit for 30 second showed the lower surface roughness average value (Ra=0.307Mm), due to their small filler particle size and their filler arrangement. The average size of nano composite filler particle is 25 nm and nano aggregates of
approximately 75 nm 23. while Composan
ceram hybrid composite finished with finishing kit for 15 second showed the
higher surface roughness average value (Ra= 0.410Mm), due to their harder and larger filler particle size 0.6 to 1 Mm 23.
Resins with a large quantity of small particles, such as Composan bio-esthetic
nano composite, investigated in this study,
reduction in size of the particles enables a better distribution in the resinous matrix. This assumption is reinforced by Reis et al
24, Nagem Filho et al 10, Turkun, Turkun 25,
who emphasized that the composite resins with higher percentage of loading and better distributed particles in the resinous matrix have greater surface smoothness. Resin composites with harder and larger filler particles like Composan ceram hybrid composite are expected to have higher Ra value after polishing. Harder filler particles are left protruding from the surface during polishing as the softer resin matrix is preferentially removed. Also this study
corroborated with Duygu et al 26, who
demonstrated that hybrid composite showed high roughness average value Ra, likely due to the size of the filler particles that were exposed after polishing or dislodge. Also in this study, it was found that there was no significant difference between the groups that finished and polished for 15 seconds and those for 30 seconds (for the same material). This result may contribute to the effectiveness of finishing kit used in this study with a relatively short polishing duration in remov-ing the scratches from the surfaces of composite resin and produced a smooth
surface. Morgan 27 reported that the ability
to produce a smooth surface with the use of the finishing kit depends on their cutting filler particles and matrix resin equally. This result came corroborate with those of Vera
et al 20, who stated that increasing the
polishing time did not result in significant improvements on surface smoothness. While, this study disagree with Tamayo et
al 17, who showed that Surface roughness
of the resin composites had a tendency to decrease with longer polishing duration.
Miyazaki et al 28, Fruits et al 29 and Yap et
al 30, reported that the polishing results
depended on the amount of time spent with each polishing system. Further studies are needed to investigate the effect of immediate and delayed finishing and polishing procedures on the surface
of different composite restorations.
Within the limits of this in vitro study; it has been found that increasing duration of finishing and polishing of the two different types of composite resins has no significant effect on the surface roughness of these two types of composite resins and there is no significant difference between these two types of composite resins in surface roughness.
1. Yazici A. Tuncer D. Antonson S. Onen A. Kilinc E. Effects of Delayed Finishing/Polishing on Sur-face Roughness, Hardness and Gloss of Tooth-Coloured Restorative Materials Eur J Dent. 2010; 4(1): 50–56
2. Peyton J. Direct restoration of anterior teeth: re-view of clinical technique and case presentation. Pract Proced Aesthet Dent 2002; 14(3): 203-210. 3. Yap A, Mok B. Surface finish of a new hybrid aes-thetic restorative material. Oper Dent 2002; 27:161-6.
4. Setcos Jm, Tarim B, Suzuki S. Surface finish pro-duced on resin composites by new polishing sys-tems. Quintessence Int 1999; 30:169-73.
5. Jung M. Finishing and polishing of a hybrid com-posite and a heat-pressed glass ceramic. Oper Dent 2002; 27:175-183
6. Rapisarda E, Bonaccorso Am, Tripi T, Torrisi L. Comparison of different finishing methods for composite and compomers. Profilometric analy-sis. Minerva Stomatol 1999; 48(5): 181-191. 7. Rapisarda E. Comparison of different finishing and
polishing techniques. Am J Dent 2000; 13(3): 136 -138.
8. Ozgunaltay G, Yazici A, Gorucu J. Effect of finish-ing and polishfinish-ing procedures on the surface roughness of new tooth-coloured restoratives. J Oral Rehabil 2003; 30 (2); 214-218.
9. Sen D, Goller G, Issever H. The effect of two pol-ishing pastes on the surface roughness of bis-acryl composite and methbis-acrylate based resins. J Prosthet Dent 2002; 88(5): 527-532.
10. Nagem Filho H, D’Azevedo M, Nagem H, Mar-sola F. Surface roughness of composite resins after finishing and polishing. Braz Dent J 2003; 14 (1): 37-41.
11. Berastequi E, Canalda C, Brau E, Miquel C. Sur-face roughness of finished composite resins. J Prosthet Dent 1992; 68(5): 742-749.
12. Yu XY, Wieczkowski G, Davis EL, Joynt RB. In-fluence of finishing technique on microleakage. J Esthet Dent 1990; 2(5): 142-144.
13. Sidhu SK, Henderson LJ. The surface finish of light-cured composite resin materials. Clin Mater
1993; 12(1): 11-15.
14.Turssi CP, de Magalhães CS, Serra MC, Rodri-gues Jr AL. Surface roughness assessment of resin-based materials during brushing proceeded by pH cycling simulations. Oper Dent 2001; 26: 576-584.
15. Cho BH, Heo SJ, Chang CG, Son HH, Kwon HC, Um CM. Colorimetric and roughness changes of ceramic blocks by polishing and glazing. Oper Dent 2001; 26: 186-192.
16. Brambilla E, Cagetti MG, Gagliani M, Fadini L, Garcia-Godoy F, Strohmenger L. Influence of different adhesive restorative materials on mu-tans streptococci colonization. Am J Dent 2005; 18(3): 173-176.
17. Tamayo W, Masahi M, Toshiki T, Hiroyasu K, Akitomo R, Susumu A. Influnce of polishing dura-tion on surface roughness of resine composites. J Oral Sci 2005; 1:21-25.
18. Cunha L G, Alonso R C, Santos P H, Sinhoreti M A. Comparative study of the surface roughness of ormocer-based and 'conventional composites. J Appl Oral Sci 2003; 11(4): 348-53.
19. Garcia F, Wang L, D’Alpino P, De Souza J, Araújo P, De Lia Mondelli R. Evaluation of the roughness and mass loss of the flowable com-posites after simulated tooth brushing abrasion. Braz Oral Res 2004; 18(2): 156-61.
20.Vera LS, Regina MP, Fabiana SN, Danielle L, Julio KUand Lornco CS. Effect of finishing and polishing techniques on the surface roughness of a nanoparticle composite resin. Braz J Oral Sci 2011; 10(2): 105-108.
21. Rustu G, Feridun H, Akin C, Ozden O, Ali K. Surface roughness of new microhybrid resin-based composites. JADA 2005; 136:1107-1112 22. Kristine GBA, Karoline GBA, Igor SM, Jose FC,
Claudia MCA. Effect of different polishing sys-tems on the surface roughness of microhybrid composits. J Appl Oral Sci 2009; 17(1): 21-26 23. Adela HG, Miguel AM, Jose CV, Amaya BE,
Pablo FG. Composite resins. A review of the materials and clinical indications. Clinical Den-tistry 2006; 11: 215-220.
24. Reis AF, Giannini M, Lovadino JR, Dias CTS. The effect of six polishing systems on the surface roughness of two packable resin-based compos-ites. Am J Dent 2002; 15(3): 193-197.
25. Turkun LS, Turkun M. The effect of one- step polishing system on the surface roughness of three esthetic composite materials. Oper Dent 2004; 29(2): 203-211.
26. Duygu S, Sinasi S, Safak k, Cagri U, Tolga K. The effect of polishing techniques on the surface roughness and color change of composite resin. J Prosthet Dent 2006; 96:33-40.
27. Morgan M. Finishing and polishing of direct pos-terior resin restorations. Pract Proced Aesthet Dent2004; 16; 211-217.
28. Miyazaki M, Yamada M, Ando S, Onose H, Kawamura h, Asano N, Sonoi S, Asao S. A
study on one- step polishing system – influence of polishing duration and hand piece load on surface texture of light – cured resins -. Nihon Shika Hozongaku Zaashi 2000; 43:1040-1049. ( in Japanese)
29. Fruits TJ, Miranda FJ, Coury TL. Effects of equivalent grit sizes utilizing differing polishing motions on selected restorative materials. Quin-tessence Int 1996; 27: 279- 285.